Cronfa - Swansea University Open Access Repository
This is an author produced version of a paper published in :
Cronfa URL for this paper:
Guo, Y. & Robertson, J. (2015). Vacancy and Doping States in Monolayer and bulk Black Phosphorus. Scientific
Reports, 5, 14165
_____________________________________________________________ This article is brought to you by Swansea University. Any person downloading material is agreeing to abide by the
terms of the repository licence. Authors are personally responsible for adhering to publisher restrictions or conditions.
When uploading content they are required to comply with their publisher agreement and the SHERPA RoMEO
database to judge whether or not it is copyright safe to add this version of the paper to this repository.
1Scientific RepoRts | 5:14165 | DOi: 10.1038/srep14165
Vacancy and Doping States in Monolayer and bulk Black PhosphorusYuzheng Guo & John Robertson
The atomic geometries and transition levels of point defects and substitutional dopants in few-layer and bulk black phosphorus are calculated. The vacancy is found to reconstruct in monolayer P to leave a single dangling bond, giving a negative U defect with a +/ transition level at 0.24 eV above the valence band edge. The V state forms an unusual 4-fold coordinated site. In few-layer and bulk black P, the defect becomes a positive U site. The divacancy is much more stable than the monovacancy, and it reconstructs to give no deep gap states. Substitutional dopants such as C, Si, O or S do not give rise to shallow donor or acceptor states but instead reconstruct to form non-doping sites analogous to DX or AX centers in GaAs. Impurities on black P adopt the 8-N rule of bonding, as in amorphous semiconductors, rather than simple substitutional geometries seen in tetrahedral semiconductors.
There has been great interest in graphene as a 2-dimensional material with a high mobility1. Unfortunately, for field effect transistor (FET) applications, it has no band gap. Another family of 2-D materials, the transition metal dichalcogenides (TMDs) such as MoS2 and WSe2, do have a band gap and are therefore useful for FETs24. However, both their valence and conduction bands are formed from transition metal d orbitals, so that the carrier mobility is not so high, ~200 cm2V1s1, much less than that of graphene4,5. In addition, their device mobilities may be limited by contact resistance problems69. Therefore, there is a desire for a stable 2D semiconductor with a band gap, large carrier mobility and ability to form good contacts with standard electrode materials.
Black phosphorous (b-P) has recently been proposed as such a 2D system1027. It has a buckled layer structure with 3-fold covalent bonding within each layer and van der Waals bonding between layers. In contrast to graphene, the lack of centre of symmetry means that b-P has a band gap. The monolayer has a direct band gap of 1.5eV, while the bulk band gap is about 0.3eV10,11. Its band edges are p states, so its carrier mobilities should be higher than those of MoS2 because p states are less sensitive to localisation than d states12,13. Field effect mobilities as high as 1000 cm2V1s1 have been reported1014 while predic-tions of hole mobilities up to 10,000 cm2 V1 s1 have been given1518. Being an elemental semiconductor, its defects might be simpler than those of binary compounds such as the TMDs. It is therefore important to determine electronic properties relevant to device performance, such as those of point defects that could trap carriers and limit field effect mobilities, or whether substitutional dopants can give shallow states to vary carrier concentrations and lower contact resistances.
Here, we calculate the band structures of few-layer black phosphorus. The energy gaps for mon-olayer and bulk are well reproduced. The electronic structure of the monovacancy is found to give rise to defects near the valence band whose configuration varies with charge state. The divacancy is found to have much lower formation energy than the monovacancy, and it reconstructs to give no deep gap states. Substitutional dopants are generally found to introduce deep defects or compensated bonding configurations, so that active shallow substitutional doping is difficult. In many ways the defect behaviour resembles that in amorphous semiconductors.
Engineering Dept, Cambridge University, Cambridge, CB2 1PZ, UK. Correspondence and requests for materials should be addressed to J.R. (email: firstname.lastname@example.org)
Received: 11 March 2015
accepted: 17 august 2015
Published: 18 September 2015
2Scientific RepoRts | 5:14165 | DOi: 10.1038/srep14165
Defect-free systemThe black P lattice consists of puckered layers, as shown in Fig. 1(a) with puckering along the Ox or armchair direction, and zigzag bonding along the Oy direction28. This structure allows considerable mechanical flexibility and very large yield strains. Along the zigzag and particularly the armchair direc-tion, strain is taken up in bond angle changes rather than bond-stretching. This leads to low elastic moduli, as bond-bending forces are less than bond-stretching forces. The hinged structure also leads to a negative Poissons ratio2831. These interesting properties also affect the defect properties. There is also a great contrast to the defect properties of graphene, where the bond-bending force constants of carbon are proportionately the highest of all group IV elements.
For the defect-free properties, the lattice constants are relaxed in both the generalised gradient approx-imation (GGA) and in the hybrid functional, and the band structure is calculated for the relaxed struc-ture. The results are compared to experiments in Table1. Figure1(bc) shows the band structure of the single layer and its density of states in screened exchange (sX). The valence band maximum (VBM) is set to be 0 eV in this figure. The calculations find that monolayer b-P has a direct gap of 1.45eV, while bulk b-P has a gap of 0.30eV. Both are in good agreement with previous experiments and calculations1622. The
Figure 1. (a) Puckered layer structure of black phosphorus, showing our color scheme to differentiate atoms in the upper and lower parts of a layer. (b) Band structure of monolayer black P, (c) Total density of states. (d) Band gap versus number of layers in few-layer black P. CNL is the charge neutrality level. (e) band alignment vs number of layers.
3Scientific RepoRts | 5:14165 | DOi: 10.1038/srep14165
PBE-style generalized gradient approximation gives a band gap of 1.0 eV for monolayer and a negative band gap for bulk b-P. Thus, the hybrid functional is necessary for electronic structure calculations of b-P.
Exciton energies are generally small in bulk 2D materials, but can become large for monolayer 2D materials, because of the lower screening32,33. A recent GW calculation of b-P suggests a large exciton energy of 0.5eV18. Interestingly, the hybrid functional is expected to give the optical gap rather than the quasi-particle gap in 2D materials34. Compared to the GW results, the flat dispersion curve at the con-duction band maximum (CBM) near along Y- is fully reproduced. Moreover, the second lowest point at CBM is in between Y and , which could be further lowered by applying strain.
Figure1(d) shows the variation of the minimum gap at with the number of layers, in good agree-ment with recent experiments35,36. The band gap E decreases as the number of layers N increases accord-ing to a power law11,22, E(N) = EB + A/Nn, where n is an index close to 1, EB is the bulk band gap and A = E(1) EB. The band gap decreases more slowly with N than it does in MoS2. The 4-layer b-P still has a band gap two times larger than the bulk value.
The charge neutrality level (CNL) is a useful reference energy that can be used to align band edges of different semiconductors and calculate Schottky barrier heights37,38. It can be calculated from the density of states (DOS). It is found to lie at 0.36 eV above the valence band edge in the monolayer case, and within the valence band for bulk b-P. We used the CNL to align the band edges of b-P for different layer numbers, as shown in Fig.1(e). We see that the valence band maximum (VBM) changes slightly less than the conduction band minimum (CBM), whereas Cai et al.22 found the reverse.
MonovacanciesNow consider the defect properties. Figure2(a) shows the ideal (unrelaxed) monovacancy in monolayer b-P. Removing one P atom leaves a dangling bond (DB) on the three adjacent P sites. Because of the lattice flexibility, the vacancy can reconstruct so that two of the DBs rebond together, as in Fig. 2(b), leaving one DB. There are two choices for rebonding, as there are two DBs on up sites and one on down sublayer sites, or vice-versa. The rebonding occurs between up and down sites, so that one defect atom now bonds to two atoms on the opposite sublayer. The reconstruction leaves adjacent 9-fold ring and 5-fold ring of bonds, Fig.2(b). This leaves one DB which can be charged + 1, 0, or 1 according to its occupancy of 0, 1 or 2 electrons.
Figure3(a) shows the relaxed geometry and the DB defect or